Epoxy self-leveling floor paint is prepared with 100% solid content of special epoxy resin as the base material. It has the excellent characteristics of green environmental protection, high gloss, one-time film thickness, paint film toughness and wear resistance. It is an ideal floor painting system for electronic enterprises, pharmaceutical enterprises, large parking lots and other places requiring high cleanliness. So what is the thickness of epoxy self-leveling floor paint? Generally speaking, the standard process thickness of epoxy self-leveling floor paint is about 1.5mm. The specific process is as follows:
1. Floor milling processing: Milling the ground with a high-speed multi-head professional ground milling machine, removing the concrete slurry on the ground surface 1-2 mm and leveling the ground. In this process, 16 milling planers are used to increase the roughness of the concrete base and the leveling of the ground. The ground is treated with a special shot blasting machine. Add grass-roots wool.2、環氧底塗：将環氧底塗材料安裝說明書配比配制并攪拌均勻，然後用滾筒均勻地滾筒于地坪表面，此工藝可以重複施工，直至完全封閉混凝土毛細孔，伸縮縫、施工縫采用貼布處理。(材料用量0.2kg/㎡，結膜厚度0mm)。
2. Epoxy primer: mix and mix the epoxy primer material in the installation instructions evenly, then use the drum to evenly roll on the surface of the floor. This process can be repeated construction until the concrete capillary holes are completely closed, and the expansion joints and construction joints are treated by sticking cloth. (Material dosage was 0.2 kg/, conjunctival thickness was 0 mm).3、砂漿中塗：在配置好的環氧中塗材料中加入一定比例的石英砂并攪拌均勻，然後用镘刀将配置好的砂漿中塗材料均勻地镘塗于完全固化後的底塗表面，待其完全固化後打磨吸塵。(材料用量0.4kg/㎡，結膜厚度0.5mm)。
3. Intermediate coating of mortar: A certain proportion of quartz sand is added into the prepared epoxy coating material and stirred evenly. Then, the coated material of the prepared mortar is uniformly coated on the fully cured surface of the undercoat with a trowel knife, and the dust is polished and cleaned after it is completely cured. (Material dosage was 0.4 kg/, conjunctival thickness was 0.5 mm).4、批塗：在配置好的環氧中塗材料中加入一定比例的碳酸鈣粉并攪拌均勻，然後用镘刀将配置好的中塗材料均勻地批塗于完全固化後的底塗表面，此工藝施工後要达到手感光滑，避免沙眼、馬蜂窩現象。(材料用量0.2kg/㎡，結膜厚度0.15mm)。
4. Batch coating: add a certain proportion of calcium carbonate powder into the prepared epoxy coating material and mix evenly. Then use a trowel knife to evenly batch the prepared coating material onto the fully cured surface of the base coating. After the construction of this process, the handle should be smooth and the trachoma and honeycomb phenomena should be avoided. (Material dosage was 0.2 kg/, conjunctival thickness was 0.15 mm).5、環氧面塗：首先将彩色面塗自流平材料按一定比例精确配置并攪拌均勻，然後用镘刀将配置好的彩色面塗材料均勻地镘塗于上工藝表面，达到顔色均勻一致，有晶面效果。(材料用量1kg/㎡，結膜厚度0.85mm)。
5. Epoxy surface coating: First, the self-leveling material of the color surface is accurately collocated and stirred evenly in a certain proportion. Then, the collocated color surface coating material is evenly coated on the upper process surface with a trowel knife to achieve uniform color and crystal surface effect. (Material dosage was 1 kg/, conjunctival thickness was 0.85 mm).當然，環氧自流平地坪漆的厚度可以根據甲方要求做成2mm、3mm等厚度，隻需要在施工時增加環氧砂漿層的厚度即可。
Of course, the thickness of epoxy self-leveling floor paint can be made into 2mm, 3mm and other thickness according to Party A's requirements, only need to increase the thickness of epoxy mortar layer during construction.
标簽:   配资盘 地坪 配资盘漆 配资盘施工 無錫配资盘